Anisotropic Li+ ion conductivity in a large single crystal of a Co(iii) coordination complex
Kim, Saet Byeol; Kim, Jeung Yoon; Jeong, Nak Cheon; Ok, Kang Min; Inorganic Chemistry Frontiers 4 (2017) 79–; doi:10.1039/C6QI00314A

data_4349536
_publ_section_title
;
 Anisotropic Li+ ion conductivity in a large single crystal of a Co(iii)
 coordination complex
;
_journal_issue                   1
_journal_name_full               'Inorganic Chemistry Frontiers'
_journal_page_first              79
_journal_paper_doi               10.1039/C6QI00314A
_journal_volume                  4
_journal_year                    2017
_chemical_formula_sum            'C14 H10 Co N2 Na O10'
_chemical_formula_weight         448.16
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_update_record
;
2016-04-24 deposited with the CCDC.
2016-10-13 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 113.564(10)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.0209(10)
_cell_length_b                   9.5023(10)
_cell_length_c                   12.8892(10)
_cell_measurement_reflns_used    3002
_cell_measurement_temperature    173.0(2)
_cell_measurement_theta_max      25.242
_cell_measurement_theta_min      2.666
_cell_volume                     1574.0(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      173.0(2)
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker SMART BREEZE'
_diffrn_measurement_method       CCD
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.073
_diffrn_reflns_Laue_measured_fraction_full 1
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            38746
_diffrn_reflns_point_group_measured_fraction_full 1
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.389
_diffrn_reflns_theta_min         2.666
_exptl_absorpt_coefficient_mu    1.184
_exptl_absorpt_correction_T_max  0.97
_exptl_absorpt_correction_T_min  0.76
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details
; 
 SADABS(Blessing, 1995) 
;
_exptl_crystal_colour            Violet
_exptl_crystal_density_diffrn    1.891
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Rod
_exptl_crystal_F_000             904
_exptl_crystal_size_max          0.137
_exptl_crystal_size_mid          0.026
_exptl_crystal_size_min          0.026
_refine_diff_density_max         0.38
_refine_diff_density_min         -0.515
_refine_diff_density_rms         0.069
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.966
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     269
_refine_ls_number_reflns         3949
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.966
_refine_ls_R_factor_all          0.0458
_refine_ls_R_factor_gt           0.0305
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0370P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0695
_refine_ls_wR_factor_ref         0.0736
_reflns_number_gt                3002
_reflns_number_total             3949
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c6qi00314a2.cif
_cod_data_source_block           NaCo
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'EMPIRICAL' was
changed to 'empirical' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/RSC/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_cell_volume        1574.1(3)
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               4349536